received: 06 April 2016 accepted: 19 May 2016 Published: 10 June 2016
Strain Engineering to Modify the Electrochemistry of Energy Storage Electrodes Nitin Muralidharan1,2, Rachel Carter2, Landon Oakes1,2, Adam P. Cohn2 & Cary L. Pint1,2 Strain engineering has been a critical aspect of device design in semiconductor manufacturing for the past decade, but remains relatively unexplored for other applications, such as energy storage. Using mechanical strain as an input parameter to modulate electrochemical potentials of metal oxides opens new opportunities intersecting fields of electrochemistry and mechanics. Here we demonstrate that less than 0.1% strain on a Ni-Ti-O based metal-oxide formed on superelastic shape memory NiTi alloys leads to anodic and cathodic peak potential shifts by up to ~30 mV in an electrochemical cell. Moreover, using the superelastic properties of NiTi to enable strain recovery also recovers the electrochemical potential of the metal oxide, providing mechanistic evidence of strain-modified electrochemistry. These results indicate that mechanical energy can be coupled with electrochemical systems to efficiently design and optimize a new class of strain-modulated energy storage materials. Traditional routes to design materials for electrochemical applications require modification of material chemical composition to control reduction-oxidation energetics when coupled with an electrolyte1,2. This causes the search for improved nanomaterials in electrochemical applications to be driven by discovery-focused nanomaterial synthesis and fabrication. Due to the complex cooperative nature of energy storage device performance based on the pairing of electrodes and electrolytes, such routes rarely lead to new materials with characteristics, such as operating voltage, that outperform existing materials. Further, whereas computational guidance has brought about a new paradigm to predict targeted material compounds that can improve advanced energy storage systems3,4, experimentalists often remain challenged by the synthesis process of such compounds, many of which are not naturally occurring. This presents a fundamental bottleneck in the conventional approach in which electrochemistry-oriented material research and development occurs that limits the rate of industry innovation in energy storage (and conversion) systems. Strain engineering, a concept widely implemented in semiconductor electronics5,6, opens new opportunities to engineer materials for electrochemical systems. The six-dimensional parameter space of the strain tensor7 enables a nanostructure with a fixed chemical composition to have electronic and physical properties finely modulated in a manner that is virtually impossible to replicate by varying chemical composition. Unlike bulk materials, many nanostructures exhibit sizes where strain can homogenously propagate throughout the whole material, instead of only on a surface or an interface6,8–14. In this spirit, recent efforts have demonstrated the capability of strain in nanostructures to modify the energy landscape of catalytic and electro-catalytic surface-bound reactions15–19 and modify oxygen ion diffusion in fuel cell technology20–22. The direct controlled correlation between mechanical strain as an input parameter and electrochemical processes in nanostructures for energy harvesting applications has only very recently been reported23. In the specific case of energy storage electrodes such as pseudocapacitors and batteries1,24, Faradaic reactions especially in metal oxides induce a change to the oxidation state of the active material often regulated by the physical characteristics of the lattice structure to enable insertion or alloying of an ion species. Focus of current research efforts so far have been on the adverse effects of strain arising from the changes to the host lattice structures during electrochemical cycling of energy storage electrodes25–27. In this regard, mechanical strain imposed onto a nanostructure leading to both physical and electronic changes that can synergistically influence energy storage redox reactions has not yet been reported despite significant advances in the ability to produce, image, and understand strain effects in materials15,28, especially those related to semiconductor electronics. Theoretical 1
Interdisciplinary Materials Science Program, Vanderbilt University, Nashville, TN 37235 USA. 2Department of Mechanical Engineering, Vanderbilt University, Nashville, TN 37235 USA. Correspondence and requests for materials should be addressed to C.L.P. (email: [email protected]
Scientific Reports | 6:27542 | DOI: 10.1038/srep27542
Figure 1. Strain engineering the surface oxide using NiTi alloy. (a) SEM image of the active NiO-TiO2 based metal oxide formed on the surface of the NiTi alloy. (b) Schematic illustration of experimental system, including the application of strain and strain recovery on a NiTi wire with surface-bound active material. (c) Stress-strain behavior of the NiTi superelastic alloy deformed up to 10% and 15% tensile strain. The dashed lines and εRE indicates the heat assisted transformation process and the recovered strain respectively. (d) DSC thermograms of the unstrained (0%) and the tensile strained (15%) states. Red (line and dots) represents the heating cycle and blue line represents the cooling cycles.
studies have recently highlighted the prospect of pre-straining materials29 even though experimental efforts in this direction remain elusive. Here we demonstrate a study where nanostructured metal oxide materials are synthesized directly on the surface of a superelastic/shapememory NiTi wire. Under the application of strain to the NiTi and transferred to the surface-bound oxides, we observe consistent shifts in the anodic and cathodic potentials. By recovering this imposed strain, we observe consistent recovery of the electrochemical potentials, clearly demonstrating that strain, as opposed to other effects, is modulating the shifts in electrochemical potentials and can be a viable tool for the design of energy storage materials.
Metal-oxide nanostructures on superelastic NiTi
A Ni-Ti-O based oxide was grown on NiTi superelastic wires at 600 °C comprising of a mixed NiO-TiO2 layer formed on top of a titanate layer on the surface of the NiTi material30,31. EDS maps (supporting information) obtained from the surface of the wire indicated a mixed Ni-Ti-O based surface oxide. Scanning electron microscopy (SEM) (Fig. 1a) was performed on the nanostructured surface oxides formed on the wire. To study strain-related modifications to energy storage processes, NiTi wires were tensile deformed to 10% and 15% strain at room temperature using an Instron mechanical testing system, with a corresponding small percentage of this input strain (less than 1%) transferred to the surface-bound oxide nanomaterial. The strained and unstrained wires with the mixed oxide layers were sonicated in peroxide at room temperature to impart nanotexturing to the oxide. This leads to a material architecture where nanostructured petals of NiO-TiO2-based metal oxides are conformally coated on the surface of a NiTi wire in a seamless manner (Fig. 1b). The Ni-Ti-O surface metal oxide was further examined through Transmission electron microscopy (TEM) (supporting information, Figure S5) indicating the crystalline nanostructure of the surface oxide. The presence of the constituent elements of the nanostructured oxide (nickel, titanium, and oxygen) was further verified using STEM EDS maps. This architecture is ideally suited to correlate strain as an input parameter to the NiTi to assess its effect on the surface-bound redox active Ni-Ti-O material for energy storage applications. The stress-strain response of the alloy is shown in Fig. 1c. The deformation behavior of the wire is described by elastic deformation of the austenite followed by the stress induced martensitic transformation below and up Scientific Reports | 6:27542 | DOI: 10.1038/srep27542
www.nature.com/scientificreports/ to 5% strain. Beyond 5% strain, oriented martensites begin to deform leading to plastic deformation of oriented martensites above 15% strain. These stress induced martensites can be transformed back to austenite by heating strained wires beyond their austenitic finish (Af ) temperatures. The final mechanical strain input onto the NiTi alloy is ~8% and 11% for tensile deformations of 10% and 15% respectively, due to the intrinsic mechanical recovery of the alloy32. Strain recovery (10% R, 15% R) in the alloy was also measured to be ~4.5% and 3.5% respectively. Differential scanning calorimetry (DSC) thermograms on 15% deformed and 0% deformed wires (Fig. 1d) demonstrates the transformation from stress induced martensite to parent austenite during the first heating cycle is present for the 15% tensile deformed wire in the temperature range of 50 to 60 °C whereas the unstrained (0%) wire showed no such transformations in this temperature range. This transformation during the first heating cycle is complete at a temperature of 60 °C which is the austenitic finish temperature (Af ). Based on the DSC results, the 15% and 10% tensile deformed alloy was heated to 60 °C in vacuum to complete the reverse transformation from stress induced martensitic state to parent austenite state. The transformation temperature around 60 °C is ideal in the case of metal oxides to avoid annealing effects which are prevalent at higher temperatures.
Spectroscopic strain analysis
As we use mechanical strain as an input parameter on NiTi to transfer strain to a surface oxide active material, XRD and Raman spectroscopy provide insight into strain transfer that enables controlled assessment of strain effects on electrochemical measurements. To characterize the transfer of strain applied to the superelastic/shapememory NiTi to the metal oxide nanostructured active material on the surface, Raman spectroscopy was carried out with 532 nm excitations (Fig. 2). The coupling of strain into a material will modify local stretch modes, hence enabling Raman spectroscopy as a sensitive tool for identifying strain in materials with distinct Raman modes. Similar to previous reports on heat treated NiTi alloys33 we find the Raman spectra of the nanostructured surface oxide to exhibit a strong peak near 269 cm−1 attributed to the titanate mode which are the Raman active modes of NiTiO334–37, peaks centered on 300 cm−1 and 342 cm−1 attributed to the Eg modes of NiTiO338–41, and a peak near 454 cm−1 attributed to the Eg mode of rutile phase TiO242,43. Whereas shifts and mode-splitting can be observed in these peaks as a function of applied strain, statistical Raman maps over large areas of the surface (800–1000 total Raman scans in each map) were performed to quantify strain-related shifts observed in the active materials, specifically for the modes identified in Fig. 2a. Lorentzian fits were applied to these Raman modes (Fig. 2b,c) and statistically validated strain effects were isolated. Upon strain recovery, these Raman modes revert back near or toward the unstrained peak positions, indicating the correlation between the measured Raman response and strain applied on the petaled nanostructured oxide surface. Importantly, the shift and reversal of the Raman modes upon strain and strain recovery across a large-area statistical sampling of the oxide without a significant bimodal or broadening effect on the peak distributions indicates the absence of interfacial delamination as a stress relief mechanism in this material system. Furthermore, the Eg mode of NiTiO3 (Fig. 2d) and TiO2 (Fig. 2e) are observed to exhibit similar recoverable shifts in the Raman modes that can be correlated with strain and straightforwardly identified. The low intensities of the observed Ni-O stretch modes44–46 near 508 cm−1 and 571 cm−1 prohibited quantitative analysis on these modes. Despite the clear signature of strain deduced through Raman spectroscopy, X-ray diffraction (XRD) provides further quantitative insight. XRD measurements indicate the same trend as Raman spectroscopy, where shifts toward lower angles are observed upon strain application, with recovery leading to the opposite shift. This is specifically shown for the (012) plane of TiO2 (Brookite) in Fig. 2f,g. To accurately determine the strain on the surface oxide using X-Ray diffractograms, Gaussian fits were applied to the obtained peaks. A standard analytical procedure was used to correlate strain to the d-spacing of the strained, unstrained, and recovered states given by the following equation, d or d R − d 0% × 100% % elastic strain = T d 0%
where, dT, dR and d0% represent the d-spacing of the tensile strained states, the recovered states and the unstrained state, respectively. This enables the strain experienced by the surface oxide to be accurately determined. The application of 10% and 15% strain to the NiTi alloy is observed to transfer ~0.04% and ~0.08% strain to the surface oxide, which can also be recovered as described in Fig. 1c. Full XRD analysis of the material is discussed in the supporting information. Strain transfer using NiTi superelastic/shapememory alloys have so far been limited to metals17 and alloys deposited on the surface with a maximum strain transfer of 2.18% achieved for an Fe-Pt metal alloy47,48. The surface oxide on the NiTi alloy, being a brittle ceramic is not as ductile as metals and metal alloys, therefore experiences cracking with less than 1% applied strain49. Overall, strain measured at